Elucidating the deprotonation of polyaniline films by X-ray photoelectron spectroscopy
Muzamir M. Mahat,abc Damia Mawad, abc Geoffrey W. Nelson,a Sarah Fearn,a Robert G. Palgrave,d
David J. Payne,a* and Molly M. Stevensabc*
a Department of Materials, Imperial College London, Exhibition Road, London SW7 2AZ,
United Kingdom b Department of Bioengineering, Imperial college London, Exhibition Road, London SW7 2AZ,
United Kingdom c Institute of Biomedical Engineering, Imperial College London, Exhibition Road, London SW7
2AZ, United Kingdom d Department of Chemistry, University College London, 20 Gordon Street, London WC1H 0AJ,
LIST OF CONTENTS:
1 Elemental composition of PANI films by XPS
2 Depth Analysis of PANI films
3 UV-Vis spectra of undoped PANI
4 Thickness of PANI films
Electronic Supplementary Material (ESI) for Journal of Materials Chemistry C.This journal is The Royal Society of Chemistry 2015
1. Elemental composition of PANI films by XPS
Fig. S1: An example of survey spectra and high resolution fitted curve of elements of pTSA-doped PANI film
at fabrication. C 1s has been fitted to have C-CH, C-N, C=N and -*. O 1s spectra fitted to have O=C and O-C.
S 2p spectra shows spin doublet which are S 2p3/2 and S 2p1/2.
Table S1: The elemental composition of PANI films at fabrication and post incubation in PBS
Film Incubation Time (hours)
0 68.3 5.1 23.2 3.4 0.5 79.8 12.6 7.6 0.05 24 81.7 12.8 5.6 0.02
0 71.9 6.5 19.8 1.8 0.5 81.9 12.1 5.9 0.1 24 80.5 11.6 7.9 0.05
Notes: Quantification done using Thermo Avantage (v. 5.948) for the C1s, N1s, O1s, and S2p3/2 peak areas; the
general curve fitting procedure can be found in the main text and by comparison to Figure S1.
2. Depth Analysis of PANI films
Fig S2: Depth analysis of S 2p signal with respect to Ar+ sputtering time for (A) pTSA and (B) CSA-doped
PANI at fabrication and following incubation in PBS for 0.5 hour and 24 hours.
3. UV-Vis spectra of undoped PANI
Fig. S3: UV-Vis spectra of undoped PANI. The spectra shows two main absorption peaks indicating benzoid
and quinoid segments at 345 nm and 592 nm, respectively. Post incubation in PBS, no changes of the absorption
spectra of PANI observed.
4. Thickness of PANI films
Table S2: The thickness of PANI films measured using surface profilometer (Dektak 150, Veeco).
Samples Incubation Time
(hours) Thickness (nm)
0.5 76.1 10.7 24 73.6 9.7
pTSA doped PANI 0 72.2 10.1
0.5 67.9 12.3 24 70.4 10.6
CSA doped PANI 0 68.1 5.6
0.5 75.0 5.1 24 78.5 10.7
Click here to load reader